# 2. Crystal Structure - Department of Physics and Astronomy crystal structure.pdf · 2. Crystal...

### Transcript of 2. Crystal Structure - Department of Physics and Astronomy crystal structure.pdf · 2. Crystal...

11

2. Crystal Structurecrystalline solid – the atoms or ions arrange in a

pattern that repeats itself in three dimensions to form a solid which has long-range order

amorphous solid – materials with only short-range order

space lattice – a network composed of an infinite three-dimensional array of points

unit cell – the repeating unit in a space lattice

lattice constantslattice vector – a, b, cinteraxial angle – α, β, γ

22

crystal system only 7 different types of unit cells14 standard (Bravais) unit cells could describe all possible lattice networks

crystal axial lengths &system interaxial angles space latticecubic a = b = c simple cubic

α = β = γ = 90o body-centered cubicface-centered cubic

tetragonal a = b≠ c simple tetragonalα = β = γ = 90o body-centered tetragonal

orthorhombic a ≠ b ≠ c simple orthorhombicα = β = γ = 90o body-centered orthorhombic

base-centered orthorhombicface-centered orthorhombic

rhombohedral a = b = c simple rhombohedralα = β = γ ≠ 90o

hexagonal a = b ≠ c simple hexagonalα = β = 90o

γ = 120o

monoclinic a ≠ b ≠ c simple monoclinicα = γ = 90o ≠ β base-centered monoclinic

triclinic a ≠ b ≠ c simple triclinicα ≠ β ≠ γ ≠ 90o

33

44

metallic crystal structures90% elemental metals crystallize into three crystal structures:․ body-centered cubic (BCC)

a (nm) R (nm)Cr 0.289 0.125Fe 0.287 0.124Mo 0.315 0.136K 0.533 0.231Na 0.429 0.186Ta 0.330 0.143W 0.316 0.137V 0.304 0.132

․face-centered cubic (FCC)a (nm) R (nm)

Al 0.405 0.143Cu 0.3615 0.128Au 0.408 0.144Pb 0.495 0.175Ni 0.352 0.125Pt 0.393 0.139Ag 0.409 0.144

․hexagonal close-packed (HCP)a c (nm) R (nm)

Al 0.2973 0.5618 0.143Zn 0.2665 0.4947 0.133Mg 0.3209 0.5209 0.160Co 0.2507 0.4069 0.125Zr 0.3231 0.5148 0.160Ti 0.2950 0.4683 0.147Be 0.2286 0.3584 0.113

55

BCC

coordination number = 8total 2 atoms per unit cell

4 R√3 a = 4 R a = ——

√3atomic packing factor (APF)

volume of atoms in unit cellAPF = ——————————

volume of unit cellAPF = 0.68

FCC

66

coordination number = 12total 4 atoms per unit cell

4 R√2 a = 4 R a = ——

√2APF = 0.74the closest packing possible of spherical atoms cubic closest-packed

HCP

coordination number = 12total 2 atoms per unit cellAPF = 0.74the closest packing possible of spherical atomsc/a ratio for ideal HCP structure is 1.633

77

the closest packing

HCP a b a b a …..

FCC a b c a b c ….

88

atom positions in cubic unit cell

BCC unit cellcoordinates of eight corners:(0, 0, 0) (1, 0, 0) (0, 1, 0) (0, 0, 1)(1, 1, 0) (1, 0, 1) (0, 1, 1) (1, 1, 1)coordinate of the center: (½, ½, ½)

direction index – the vector components of the direction resolved along each of the coordinate axes and reduced to the smallest integers

all parallel direction vectors have the same direction indices

99

directions are crystallographically equivalent if the atom spacing along each direction is the same

ex. cubic edge directions:[100] [010] [001] [010] [001] [100]≣ <100>

equivalent directions are called indices of a family or form

ex. draw the following directions: (a) [112]

(b) [110]

(c) [321]

1010

Miller indices for crystallographic planesMiller notation system (hkl)Miller index – the reciprocals of the fractional

intercepts that the plane makes with the x, y, and z axes of the three nonparallel edges of the cubic unit cell

procedure for determining Miller index:(1) choose a plane not pass through (0, 0, 0)(2) determine the intercepts of the plane with

x, y, and z axes (3) form the reciprocals of these intercepts(4) find the smallest set of whole numbers

that are in the same ratio as the interceptsex.

1111

ex. draw the following crystallographic planes in cubic unit cell:

(a) (101) (b) (110)

(c) (221)

planes of a family or form {hkl}ex. (100), (010), (001) are a family

{100}an important relationship for cubic system, the direction indices of a direction perpendicular to a crystal plane are the same as the Miller indices of that plane

1212

interplanar spacing between two closest parallel planes with the same Miller indices is designated dhkl (h, k, l are the Miller indices)

adhkl = ——————

√h2 + k2 + l2

a: = lattice constant

ex. determine the Miller indices of the planes shown as follow:

(a) (b)

(5120) (646)

1313

hexagonal structureMiller-Bravais indices – HCP crystal plane

indices (hkil) h + k + i = 0three basal axes a1, a2, a3 and c axis

basal planes (0001)prism planes

(ABCD) (1010)

(ABEF) (1100)

(CDGH) (0110)

1414

direction indices in HCP unit cellfour indices [uvtw] u + v + t =0

u = ⅓(2u – v) v = ⅓(2u – v) t = -(u + v)directions a1, a2, a3

+a3 direction incorporating c axis

directions on the upper basal planes

15

volume, planar, linear densityvolume density

mass/unit cellρv = ————————

volume/unit cellex. Cu has FCC structure, atomic radius of

0.1278 nm, atomic mass of 63.54 g/molcalculate the density of Cu in Mg/m3.

FCC structure √2 a = 4 Ra = 2 √2 R = 2 √2 (1.278 × 10-10)

= 3.61 × 10-10mV = (3.61 × 10-10 m)3 = 4.70 × 10-29 m3

4 Cu per unit cellm = 4 × 63.54 × 1.66 × 10-30 Mg = 4.22 × 10-28 Mgρv = 4.22 × 10-28 Mg / 4.70 × 10-29 m3

= 8.98 Mg/m3 (exp. = 8.96 Mg/m3 )

planar atomic densityequiv. no. of atoms whose centers

are intersected by selected areaρp = ————————————

selected areaex. calculate planar atomic density ρp on (110)

plane of the α-Fe in BCC lattice in atoms/mm2. (lattice constant a = 0.287 nm)

15

16

1 atom (center) + ¼ atom (corner) × 4 = 2 atomsarea = a × √2 a = √2 a2 = √2 (2.87 × 10-7)2

= 1.164 × 10-13 mm2

2 atomsρp = ———————— = 1.72 × 1013 atoms/mm2

1.164 × 10-13 mm2

linear atomic densityno. of atoms diam. intersected by selected

length of line in direction of interestρl = ———————————————

selected length of line ex. calculate linear atomic density ρl in [110]

direction in Cu crystal lattice in atoms/mm. (Cu is FCC and lattice constant a = 0.361 nm)

16

17

no. of atoms = ½ + 1 + ½ = 2 atomslength = √2 a = √2 (3.61 × 10-7)

= 5.104 × 10-7 mm 2 atoms

ρl = ——————— = 3.92 × 106 atoms/mm 5.104 × 10-7 mm

polymorphism or allotropyelement or compound exists in more than one crystalline form under different conditions of temperature and pressureex.

crystal structure at othermetal at room temperature temperature 1

Ca FCC BCC (> 447oC)Co HCP FCC (> 427oC)Hf HCP BCC (> 1742oC)Fe BCC (α) FCC (912-1394oC) (γ)

BCC (> 1394oC) (δ) Li BCC HCP (< -193oC)Na BCC HCP (< -233oC)Tl HCP BCC (> 234oC)Ti HCP BCC (> 883oC) Y HCP BCC (> 1481oC) Zr HCP BCC (> 872oC) 1

17

18

crystal structure analysisX-ray sources

x-rays used for diffraction are radiations with wavelengths 0.05 ~ 0.25 nm

a voltage of 35 kV is applied between cathode (W filament) and anode (Mo target)

x-ray spectrum 0.2 ~ 1.4 nmwavelength of Kα line 0.07 nm

18

19

X-ray diffractionreflected wave patterns of beam are not in phase, no reinforced beam will be produceddestructive interference occurs

reflected wave patterns of beam are in phase, reinforcement of the beam or constructive interference occurs

nλ = MP + PN n = 1, 2, 3…..nλ = 2 dhkl sinθ 19

2020

ex. BCC Fe placed in an x-ray diffractometerusing x-ray with λ = 0.1541 nm. diffraction from {110} planes was obtained at 2θ = 44.704o. calculate lattice constant a.

λ = 2 d110 sinθλ 0.1541 nm

d110 = ——— = —————— = 0.2026 nm2sinθ 2sin(22.352o)

a = dhkl √h2 + k2 + l2 = 0.2026√2 = 0.287 nm

X-ray diffraction analysis of crystal structurespowder diffraction methoddiffractometer

2121

diffraction pattern for cubic unit cella

dhkl = —————— and λ = 2d sinθ√h2 + k2 + l2

2 a sinθλ = ———————

√h2 + k2 + l2

rules for determining the diffracting {hkl} planes in cubic crystals

reflection present reflection absentBCC (h + k + l) = even (h + k + l) = oddFCC (h, k, l) all odd or (h, k, l) not all odd

all even or all evenex. Diffraction pattern for W sample by the

use of a diffractometer with Cu radiation

W : BCC structure

22

2 a sinθλ = ——————

√h2 + k2 + l2

λ2(h2 + k2 + l2)sin2θ = ———————

4a2

sin2θA h2A + k2

A + l2A——— = ———————

sin2θΒ h2B + k2

B + l2B

Miller indices of the diffracting planes for BCC and FCC{hkl} Σ[h2 + k2 + l2 ] FCC BCC{100} 1 ….. …..{110} 2 ….. 110{111} 3 111 …..{200} 4 200 200{210} 5 ….. …..{211} 6 ….. 211

first two sets of diffraction planesFCC {111) and {200}sin2θA h2

A + k2A + l2

A——— = ——————— = 0.75sin2θΒ h2

B + k2B + l2

B

23

BCC {110) and {200}sin2θA h2

A + k2A + l2

A——— = ——————— = 0. 5sin2θΒ h2

B + k2B + l2

Bex. an element that has either BCC or FCC

structure shows diffraction peaks at following 2θ angles: 40, 58, 73, 86.8, 100.4 and 114.7. wavelength of x-ray λ = 0.154a. BCC or FCC?b. determine the lattice constant a.c. identify the element.

(a) 2θ θ sinθ sin2θ40 20 0.3420 0.117058 29 0.4848 0.235073 36.5 0.5948 0.353886.8 43.4 0.6871 0.4721

100.4 50.2 0.7683 0.5903first and second angles0.1170/0.3420 = 0.5 BCC structure

(b) λ √h2 + k2 + l2 0.154 √2a = — —————— = ——— ———

2 sinθ 2 0.342= 0.318 nm

(c) W